Next Generation Ceramic Substrate Fabricated at Room Temperature Yuna Kim1,2, Cheol-Woo Ahn1, Jong-Jin Choi1, Jungho Ryu1, Jong-Woo Kim1, Woon-Ha Yoon1, Dong-Soo Park1, Seog-Young Yoon2, Byungjin Ma3 & Byung-Dong Hahn1
Received: 16 March 2017 Accepted: 16 June 2017 Published: xx xx xxxx
A ceramic substrate must not only have an excellent thermal performance but also be thin, since the electronic devices have to become thin and small in the electronics industry of the next generation. In this manuscript, a thin ceramic substrate (thickness: 30–70 µm) is reported for the next generation ceramic substrate. It is fabricated by a new process [granule spray in vacuum (GSV)] which is a room temperature process. For the thin ceramic substrates, AlN GSV films are deposited on Al substrates and their electric/thermal properties are compared to those of the commercial ceramic substrates. The thermal resistance is significantly reduced by using AlN GSV films instead of AlN bulk-ceramics in thermal management systems. It is due to the removal of a thermal interface material which has low thermal conductivity. In particular, the dielectric strengths of AlN GSV films are much higher than those of AlN bulk-ceramics which are commercialized, approximately 5 times. Therefore, it can be expected that this GSV film is a next generation substrate in thermal management systems for the high power application. Ceramic materials for thermal management have gained considerable attention in the electronics industry, since the life and performance of electronic devices are dependent on the heat dissipation of electronic packages1–8. In general, a thermal management system consists of a ceramic substrate, a thermal interface material (TIM), and a heat sink (Al) as indicated in the left figure of Fig. 1. Among the materials, a TIM has the thermal conductivity much lower than the others5. In particular, a ceramic substrate must be thin, since the electronic devices have to become thin and small in the electronics industry of the next generation. Hence, we report the electric and thermal properties of AlN films which were directly coated on Al substrate without a TIM layer. AlN is the ceramic material which has high conductivity (100–270 W/mK) and it is used for a ceramic substrate in the electronics industry6. The AlN film had better be deposited at room temperature (RT), since the heat treatment is limited due to the easy oxidation and the low melting point (approximately 660 °C) of Al. Therefore, we designed the granule spray in vacuum (GSV) which was the room temperature process to fabricate thick films. In this study, we report what GSV is and why GSV is required. In addition, the electric and thermal properties of AlN GSV films, deposited on Al substrates, are compared to those of commercialized structures (fabricated with bulk-AlN ceramics).
Process Design of Granule Spray in Vacuum (GSV). The AD method is an interesting technology which is used to fabricate a dense film at room temperature7–17. The fine particles, which are accelerated by an air compressor, are ejected through the nozzle and collide onto the substrate with high speed as shown in Fig. 2(a). Owing to the fracture and plastic deformation of fine particles, the dense ceramic film is formed at room temperature (RT)14–17. It is interesting that the dense film is formed without any heat treatment at an AD process. The AD film shows the interesting characteristics, such as the dense microstructure, nano-size grains, the high deposition speed (approximately 1–10 min for the thickness of 1 μm and the area of 10 × 10 cm2), the wide thickness range (from submicron to hundreds micrometers), the easy manufacture of composite films and multi-layers, the easy manufacture of flexible films (through the usage of flexible substrates), and no use of heat treatment for densification16. Compared to the other methods such as sputtering and pulsed laser deposition (PLD), the deposition 1
Functional Ceramics Department, Korea Institute of Materials Science, 797 Changwon-daero, Seongsan-gu, Changwon, Gyeong-Nam, 51508, Republic of Korea. 2School of Materials Science and Engineering, Pusan National University, 2, Busandaehak-ro 63beon-gil, Geumjeong-gu, Busan, 46241, Republic of Korea. 3Reliability Research Center, Korea Electronics Technology Institute, 25, Saenari-ro, Bundang-gu, Seongnam-si, Gyeonggi-do, 13509, Republic of Korea. Correspondence and requests for materials should be addressed to C.-W.A. (email: [email protected]
kims.re.kr) or B.-D.H. (email: [email protected]
) Scientific REPOrTS | 7:6637 | DOI:10.1038/s41598-017-06774-z
Figure 1. Schematic diagram of heat flow at substrate structures with TIM and without TIM. The removal of a TIM layer can improve the thermal dissipation in thermal management systems.
speed of an AD method is significantly high. In addition, the grains are randomly oriented, while a PLD film shows epitaxial growth. In particular, an AD method is a room temperature process. It has been reported that an AD film could be used for the various applications (piezoelectric devices, sensors, bio-devices, batteries, ceramic substrates etc.)7, 8, 14–17. However, the technology is not completed yet. In particular, the continuous flow of aerosol must be guaranteed to fabricate a uniform film using the AD method. As indicated in the left figure of Fig. 2(b), however, a lump of powder is formed at the bottleneck of a powder feeder with ease and it interferes with the aerosol flow in the AD equipment. Hence, the lump of powder must be removed for this AD method to be commercialized. The powder lump is formed due to the large surface area of fine particles. Therefore, GSV has been designed to improve the aerosol flow as seen in the right figure of Fig. 2(b). When the films are deposited by GSV, the lump of powder is not observed. At the GSV process, granules are used instead of fine particles as seen in Fig. 2(b). In order to obtain the fracture and plastic deformation of primary particles, high kinetic energy is essential in the AD method. When the particles collide onto the substrate with high speed, they are fractured to be nano-size particles and their surface area is dramatically increased. Owing to this high surface energy and the instantaneous surface temperature of 500–1000 °C, the densification of an AD film occurs, when the other particles collide onto these nano-size particles with high speed, as shown in Fig. 2(c). It has been reported that the instantaneous surface temperature of particles and a substrate can be approximately 500–1000 °C when the particles collide onto the substrate with high speed (approximately 150–500 m/s)14. In general, hence, the film of a material which has a low sintering temperature is easy to be deposited in an AD or GSV process. In addition, the compaction of the fractured particles occurs due to the continuous impact of fine particles and it can assist the densification of the AD film. During this compaction process, the sub-micron-size particles are frequently trapped in AD films, as shown in Fig. 2(c). The fine particles must be fractured by their kinetic energy for AD films to be deposited on the substrates, as explained above. If the kinetic energy is not enough for the particles to be fractured (due to the light mass or the low speed of particles), the particles will not be fractured as shown in the top figure of Fig. 3(a). The light mass means the small particle in Fig. 4(a). On the contrary, the surface of a substrate can be peeled by the high impact energy of large particles, when the kinetic energy is immoderate (owing to the heavy mass or the high speed of particles). Even though the particles are fractured, the size of fractured particles is too large to be deposited on the substrate, as indicated in the middle figure of Fig. 3(a). In order to be well-deposited on the substrate, the fractured particles must be nano-sized as explained above. Although the small amount of nano-size particles can be existed on a substrate, they are easily removed by the continuous impact of large fine-particles. Therefore, the optimum size and velocity of fine particles must be used for the AD films to be successfully deposited, as marked with the blue color in Fig. 4(a). A gray area is the forbidden zone in which the film is not deposited. The optimum condition is dependent on the kind of materials. When the conditions are satisfied, the AD films are deposited as shown in the bottom figure of Fig. 4(a). This AD process must be significantly improved as shown in Fig. 2(b), although the AD films can be deposited by considering those conditions. The continuous flow of aerosol can be guaranteed by using granules instead of fine particles, as mentioned above. The granules consist of the fine particles which have the optimum size as exhibited in the bottom figure of Fig. 3(b). In the GSV process, the deposition of GSV films is dependent on the fracture of primary particles. The surface of a substrate can be peeled due to the high impact energy of large granules, if the primary particles cannot be fractured by the impact of granule as shown in the top figure of Fig. 3(b). This hard granule is formed by the strong bonding among primary particles. Therefore, the primary particles must be weakly bonded to be easily fractured, in the fragile granules, for the GSV films to be deposited on a substrate as shown in the bottom figure of Fig. 3(b). The bonding strength (among primary particles) can be controlled by the annealing temperature of granules as seen in Fig. 4(b). The higher temperature means the harder granule. The difference of the bonding strength was measured as indicated in the inset of Fig. 4(b). As shown in Fig. 4(b), the granules did not show the significant difference at the SEM images, but their bonding strengths were severely different. The granules, hence, which were heat-treated at 800 °C, might be well-fractured at a GSV process, while they could not be well-fractured when they were heat-treated at 1000 °C. Owing to this tendency of fracture, the AlN GSV films could be well-formed on the Al substrate, when the granules were heat-treated at 800 °C. In general, the optimum temperature is also dependent on the kind of materials and the size of primary particles. Scientific REPOrTS | 7:6637 | DOI:10.1038/s41598-017-06774-z
Figure 2. Difference between AD and GSV: (a) overall equipment, (b) bottleneck of aerosol chamber, and (c) deposition behavior. A lump of powders is not formed in a GSV process. For film deposition, the fine particles must be fractured to be nano-size. The compaction of particles can assist the densification of films. The film thickness is dependent on the portion of trapped sub-micron grains.
In general, as seen in Fig. 4(a), the coating condition is wider in a GSV process than in an AD process, although the difference is not significant. The difference is due to the size distribution of fractured particles. The granules have the kinetic energy much higher than fine particles, owing to their heavy masses. This high kinetic energy is principally consumed by the fracture of a fragile granule. In addition, the fracture of primary particles occurs from the particles which are close by the impact surface. Therefore, the size distribution of fractured particles is wider in a GSV process than in an AD process. This wide size distribution of fractured particles makes the Scientific REPOrTS | 7:6637 | DOI:10.1038/s41598-017-06774-z
Figure 3. Deposition behaviors in (a) AD and (b) GSV. The AD films can be formed by using the optimum particle size. The GSV films can be formed by using the fragile granules. coating condition wider as shown in Fig. 4(a). Furthermore, the trapped sub-micron particles [Fig. 2(c)] are also observed in GSV films more than in AD films. Owing to the huge size of granules [compared to fine particles, as shown in Fig. 2(c)] and the wide size distribution of fractured particles, the sub-micron particles can have chance to be trapped among the nano-size particles in a GSV process more than in an AD process. For the compaction of the fractured particles, granules are also more effective than fine particles.
Crystal Structure and Microstructure of AlN GSV Film. Figure 5 shows the X-ray diffraction (XRD) patterns of AlN powders (heat-treated at 800 °C and 850 °C in air) and AlN films (AD and GSV, deposited on Al substrates). As seen in Fig. 5(a), the Al2O3 peaks were not detected at the XRD patterns, when AlN powers were heat-treated at 800 °C (AlN 800). On the contrary, they were found at the XRD patterns of the AlN powders which were heat-treated at 850 °C (AlN 850). The peak intensity for AlN decreased with the rise of heat-treatment temperature as seen in the inset of Fig. 5(a). Moreover, the peaks of Al2O3 were detected at AlN 850. Hence, the surface of AlN 800 might be also oxidized, although the oxidation rate was negligible. In an AD process, AlN 850 had to be used for the AlN AD films to be well-deposited on an Al substrate. Using AlN 800, it was difficult to obtain the thick AlN AD film which was thicker than 10 µm. In addition, we have tried to deposit the AlN AD films using pure AlN powders after controlling their particle sizes and phases (no Al2O3, heat-treated in N2 and H2 atmosphere), and then the film thickness was limited to be